# SECOND ORDER PHASE FIELD ASYMPTOTICS FOR MULTI-COMPONENT ... SECOND ORDER PHASE FIELD ASYMPTOTICS...

date post

09-Apr-2020Category

## Documents

view

3download

0

Embed Size (px)

### Transcript of SECOND ORDER PHASE FIELD ASYMPTOTICS FOR MULTI-COMPONENT ... SECOND ORDER PHASE FIELD ASYMPTOTICS...

SECOND ORDER PHASE FIELD ASYMPTOTICS

FOR MULTI-COMPONENT SYSTEMS

HARALD GARCKE AND BJÖRN STINNER

Abstract. We derive a phase field model which approximates a sharp interface model for solidification of a multicomponent alloy to second order in the interfacial thickness ε. Since in numerical computations for phase field models the spatial grid size has to be smaller than ε the new approach allows for considerably more accurate phase field computations than have been possible so far.

In the classical approach of matched asymptotic expansions the equations to lowest order in ε lead to the sharp interface problem. Considering the equations to the next order, a correction problem is derived. It turns out that, when taking a possibly non- constant correction term to a kinetic coefficient in the phase field model into account, the correction problem becomes trivial and the approximation of the sharp interface problem is of second order in ε. By numerical experiments, the better approximation property is well supported. The computational effort to obtain an error smaller than a given value is investigated revealing an enormous efficiency gain.

1. Introduction

In sharp interface approaches to solidification phase boundaries are modelled as hyper- surfaces across which certain quantities jump. In the last two decades also the phase field method has become a powerful tool for modelling the microstructural evolution during solidification (see [7, 25, 11, 8] for reviews). Instead of explicitly tracking the solid-liquid interface an order parameter is used. It takes different values in the phases and changes smoothly in the interfacial regions which leads to the notion of diffuse interface models. The typical thickness of the diffuse interface is related to a small parameter ε. In the limit as ε → 0 sharp interface models are recovered.

The relation between the phase field model and the free boundary problem is established using the method of matched asymptotic expansions. It is assumed that the solution to the phase field model can be expanded in ε-series in the bulk regions occupied by the phases (outer expansion) and, using rescaled coordinates, in the interfacial regions (inner expansion). To leading order in ε, a sharp interface problem is obtained. If we consider the phase field system as an approximation of the sharp interface problem it would of course be desirable that phase field solutions converge fast with respect to ε to solutions to the sharp interface problem. This becomes even more important as in numerical computations the spatial grid size has to be chosen smaller than ε (see e.g. [14]). In this paper we are interested in phase field approximations of the sharp interface problem which are of second order, i.e., we aim for constructing phase field systems such

Date: September 7, 2005. 1991 Mathematics Subject Classification. 82C26, 82C24, 35K55, 34E05, 35B25, 35B40, 65M06. Key words and phrases. phase field models, sharp interface models, numerical simulations, matched

asymptotic expansions.

1

that the first order correction in the ε-expansion vanishes. This would then lead to much more efficient numerical approaches for solidification.

The method is formal in the sense that, a posteriori, it is not controlled whether the asymptotic expansions really exist and converge. In the context of solidification it has been applied on models for pure substances [10, 26], alloys [30, 5], multi-phase systems [16], and systems with both multiple phases and components [17] in order to derive sharp interface limits (first order asymptotics). We remark that, in some cases, this ansatz has been verified by rigorously showing that, in the limit as ε → 0, the sharp interface model is obtained from the diffuse interface model (see e.g. [1, 10, 12, 28]).

Our interest in the higher order approximation is motivated by the results obtained by Karma and Rappel [20] in the context of thin interface asymptotics where the interface thickness is small but remains finite. Their analysis led to a positive correction term in the kinetic coefficient of the phase field equation balancing undesirable O(ε)-terms in the Gibbs-Thomson condition and raising the stability bound of explicit numerical methods. Besides, the better approximation allows for larger values of ε and, therefore, for coarser grids. In particular, it is possible to consider the limit of vanishing kinetic undercooling. Almgren [2] extended the analysis to the case of different diffusivities in the phases and discussed both classical asymptotics and thin interface asymptotics. By choosing different interpolation functions for free energy density and internal energy density an approximation to second order can still be achieved but the gradient structure of the model and thermo- dynamical consistency are lost. Andersson [4] showed, based on the work of Almgren, that even an approximation of third order is possible by using high order polynomials for the interpolation. McFadden, Wheeler, and Anderson [24] used an approach based on an en- ergy and an entropy functional providing more degrees of freedom to tackle the difficulties with unequal diffusivities in the phases while avoiding the loss of the thermodynamical consistency. Again, both classical and thin asymptotics are discussed as well as the limit of vanishing kinetic undercooling. In a more recent analysis Ramirez et al. [27] considered a binary alloy also involving different diffusivities in the phases and obtained a better ap- proximation by adding a small additional term to the mass flux (antitrapping mass current, the ideas stem from [19]).

We aim to extend the results to general non-isothermal multi-component alloy systems allowing for arbitrary phase diagrams with two phases. The models studied in the literature usually use the free energy or the entropy as thermodynamical potentials (see e.g. [3, 26, 29, 30] and the discussion in [21]). It turns out that, in our context, the reduced grand canonical potential ψ (see [23]) is more appropriate for the analysis. To motivate this let us review some thermodynamics.

We will, for simplicity, consider a system with uniform density, which is in mechanical equilibrium throughout the evolution. Changes is pressure or volume are neglected. In this case, the Helmholtz free energy density f is an appropriate thermodynamical quantity to work with. It is conveniently written as a function of the absolute temperature T and the concentrations c = (c(1), . . . , c(N)) ∈ RN , its derivatives being the negative entropy density −s and the chemical potentials µ = (µ(1), . . . , µ(N)) ∈ RN ,

df = −s dT + µ · dc.

Here, the central dot denotes the scalar product on RN . The internal energy density is e = f + Ts. For the reduced grand canonical potential ψ = − g

T , g = f − µ · c being the

2

grand canonical potential, we then obtain

dψ = d (f − µ · c

−T )

= e d (−1

T

)

+ c · d (µ

T

)

,

in particular u = (u(0), ũ) = (−1 T

, µ T ) ∈ RN+1 are the to (e, c) ∈ RN+1 conjugated variables.

Assuming local thermodynamical equilibrium the vector u is continuous across the free boundary in a sharp interface model. This will be important in the matched asymptotic expansions studied later and therefore we will state the problem from the beginning in these variables. We refer to Appendix A for more details on the thermodynamical background.

Next, we will briefly state a sharp interface problem for a liquid-solid phase change in a non-isothermal multi-component system (cp. [17] for more details). Let Dl and Ds be the domains occupied respectively by the liquid phase and the solid phase and let Γ be the interface separating the phases. In Dl and Ds, conservation of mass and energy is expressed by the balance equations

∂tψ,u(i)(u) = −∇ · Ji = −∇ · N∑

j=0

Lij∇(−u(j)), 0 ≤ i ≤ N, (1)

where ψ,u(0) = e and ψ,u(i) = c (i) denote derivatives of ψ, the Ji are the fluxes, and L =

(Lij)i,j is a matrix of Onsager coefficients which may depend on u. Constitutive relations between ψ, L, and u may depend on the two phases s and l. On Γ it holds

u(i) is continuous, 0 ≤ i ≤ N, (2)

[−Ji]ls · ν = [

− N∑

j=0

Lij∇u(j) ]l

s · ν = v[ψ,u(i)(u)]ls, 0 ≤ i ≤ N, (3)

αv = σκ − [ψ(u)]ls, (4)

where ν is the unit normal on Γ pointing into Dl, v is the normal velocity into the direction ν, σ is the surface tension, κ the curvature, α a kinetic coefficient, and [·]ls denotes the jump of the quantity in the brackets, for example [ψ(u)]ls = ψl(u) − ψs(u). Equations (2) and (3) are also due to conservation of mass and energy. The Gibbs-Thomson conditions (4) couples the motion of the phase boundaries to the thermodynamical quantities of the adjacent phases such that, locally, entropy production is non-negative. For the case of a system involving multiple phases this is shown in [17].

The above stated sharp interface model will be approximated by a phase field model of the form

ω∂tϕ = σ∆ϕ − σ 1ε2 w ′(ϕ) + 1

2ε h′(ϕ)

( ψl(u) − ψs(u)

) , (5)

∂tψ,u(i)(u, ϕ) = ∇ · N∑

j=0

Lij∇u(j), 0 ≤ i ≤ N. (6)

Here, ϕ is the phase field variable. We have ϕ = 1 in the liquid phase and ϕ = 0 in the solid phase. The function w is a double-well potential with minima in 0 and 1 corresponding to the values of ϕ in the pure phases. The reduced grand canonical potentials ψl and ψs of the pure phases are interpolated to ob

*View more*